Influence of Solvents and Composition of Etch-and-Rinse and Self-Etch Adhesive Systems on the Nanoleakage within the Hybrid Layer
Joao Cardoso Ferreira, Patricia Teixeira Pires, Alvaro Ferreira Azevedo, Sofia Arantes Oliveira, Paulo Ribeiro Melo, Mario Jorge Silva
Citation Information :
Ferreira JC, Pires PT, Azevedo AF, Oliveira SA, Melo PR, Silva MJ. Influence of Solvents and Composition of Etch-and-Rinse and Self-Etch Adhesive Systems on the Nanoleakage within the Hybrid Layer. J Contemp Dent Pract 2013; 14 (4):691-699.
The goal of this study was to evaluate nanoleakage within the hybrid layer yielded by etch-and-rinse and self-etch adhesive systems, with different solvents and compositions.
Materials and methods
Four adhesives were applied onto 20 human dentin disks: group A: Adper Scotchbond 1XT™ (3M ESPE), group B: One Coat Bond® (Coltène Whaledent), group C: AdheSE® (Ivoclar Vivadent) and group D: Xeno-V® (Dentsply). The samples were immersed in aqueous ammoniacal silver nitrate for 24 hour, prepared and observed under field-emission scanning electron microscopy with backscattered electrons. Microphotographs were scanned and data were processed. The mean value and standard deviation were calculated. KruskalWallis and Mann-Whitney tests were used (p < 0.05).
All the adhesives showed nanoleakage within the hybrid layer: Adper Scotchbond 1XT™ (218.5 μm ± 52.6 μm), One Coat Bond® (139.6 μm ± 79.0 μm), AdheSE® (92.7 μm ± 64.8 μm) and Xeno-V® (251.0 μm ± 85.2 μm). AdheSE® yielded less nanoleakage than Adper Scotchbond-1XT™ (p = 0.003) and than Xeno-V® (p = 0.007). No other statistically significant differences were detected.
Two-step self-etch adhesive system (AdheSE®) might contribute for lower nanoleakage deposition and thus better performance in dentin adhesion.
The two-step self-etch adhesive system showed the lowest nanoleakage deposition compared with the other adhesive systems evaluated, which seems to indicate a better behavior when a restoration is performed in dentin and possibly can lead to a durable adhesion along time.
How to cite this article
Ferreira JC, Pires PT, Azevedo AF, Oliveira SA, Melo PR, Silva MJ. Influence of Solvents and Composition of Etch-and-Rinse and Self-Etch Adhesive Systems on the Nanoleakage within the Hybrid Layer. J Contemp Dent Pract 2013;14(4):691-699.
Qualitative analysis of adhesive interface nanoleakage using FE-SEM/EDS. Dent Mater 2007;23:561-569.
Nanoleakage: leakage within the hybrid layer. Oper Dent 1995;20:18-25.
Effect of primer apllication on dentin permeability. Iowa: University of Iowa 2004;6-8
Effect of mode of conditioning treatment on efficacy of dentin bonding. Oper Dent 1996;21:31-35.
Nanoleakage types and potential implications: evidence from unfilled and filled adhesives with the same resin composition. Am J Dent 2004;17:182-190.
Permeability of marginal hybrid layers in composite restorations. Clin Oral Investig 2005;9:1-7.
Nanoleakage within the hybrid layer: A correlative FEISEM/TEM investigation. J Biomed Mater Res B Appl Biomater 2005;73:7-14.
Two modes of nanoleakage expression in single-step adhesives. J Dent Res 2002;81:472-476.
Interaction patterns between dentin and adhesive on prepared class V cavities in vitro and in vivo. J Biomed Mater Res 2000;53:86-92.
Effects of storage media on mechanical properties of adhesive systems. Am J Dent 2004;17:104-108.
Degradation patterns of different adhesives and bonding procedures. J Biomed Mater Res B Appl Biomater 2003;66:324-330.
The effect of a self-etching primer on the continuous demineralization of dentin. Eur J Oral Sci 2004;112:376-383.
Interfacial ultramorphology of single-step adhesives: nanoleakage as a function of time. J Oral Rehabil 2007;34:213-221.
Water sorption/solubility of dental adhesive resins. Dent Mater 2006;22:973-980.
A challenge to the conventional wisdom that simultaneous etching and resin infiltration always occurs in selfetch adhesives. Biomaterials 2005;26:1035-1042.
Dental adhesion: present state of the art and future perspectives. Quintessence Int 2002;33:213-224.
Effects of the acetone content of single solution dentin bonding agents on the adhesive layer thickness and the microtensile bond strength. Dent Mater 2004;20:107-115.
A confocal microscopic evaluation of resin-dentin interface using adhesive systems with three different solvents bonded to dry and moist dentinan in vitro study. Quintessence Int 2005;36:511-521.
Effect of solvent and rewetting time on dentin adhesion. Quintessence Int 2001;32:385-390.
How wet should dentin be? Comparison of methods to remove excess water during moist bonding. J Adhes Dent 2001;3:257-264.
Dentin bond strengths as a function of solvent and glutaraldehyde content. Am J Dent 2001;14:221-226.
Effect of primer solvent and curing mode on dentin shear bond strength and interface morphology. Quintessence Int 2003;34:548-555.
Morphological characterization of single bottle adhesives and vital dentin interface. Am J Dent 2002;15:31-34.
A 36-month clinical evaluation of ethanol/water and acetone-based etch-and-rinse adhesives in non-carious cervical lesions. Oper Dent 2009;34:384-391.
Water movement in the hybrid layer after different dentin treatments. Dent Mater 2004;20:796-803.
Resin-dentin interfacial ultrastructure and microtensile dentin bond strength after five-year water storage. Oper Dent 2004;29:705-712.
Field emission SEM comparison of four postfixation drying techniques for human dentin. J Biomed Mater Res 1995;29:1111-1120.
Effect of aging on dentin bonding. Am J Dent 1993;6:145-147.
Variability in microleakage observed in a total-etch wet-bonding technique under different handling conditions. J Dent Res 1995;74:1168-1178.
Comparative SEM and TEM observations of nanoleakage within the hybrid layer. Oper Dent 1995;20:160-167.
Active application improves the bonding performance of self-etch adhesives to dentin. J Dent 2009;37:82-90.
Relationship between microtensile bond strength and nanoleakage at the composite-dentin interface. Dent Mater 2009;25:135-141.
Adhesive phase separation at the dentin interface under wet bonding conditions. J Biomed Mater Res 2002;62:447-456.
Micromorphological spectrum from overdrying to overwetting acid-conditioned dentin in waterfree acetone-based, single-bottle primer/adhesives. Dent Mater 1996;12:236-244.
Current aspects on bonding effectiveness and stability in adhesive dentistry. Aust Dent J 2011;56 Suppl 1:31-44.
Estudo comparativo da infiltração marginal com duas “gerações” de adesivos: total-etch em sistema monofrasco versus sistema self-etching. Porto: Faculdade de Medicina Dentária da Universidade do Porto 2004;25-26, 67-72
Hydrolytic stability of self-etching adhesive systems. J Adhes Dent 2005;7:107-116.
State of the art etch-andrinse adhesives. Dent Mater 2011;27:1-16.
Ultramorphological analysis of resin-dentin interfaces produced with water-based single-step and two-step adhesives: nanoleakage expression. J Biomed Mater Res B Appl Biomater 2004;71:90-98.
The in vitro dentin bond strengths of two adhesive systems in class I cavities of human molars. J Adhes Dent 2002;4:31-39.
Buonocore memorial lecture. Adhesion to enamel and dentin: current status and future challenges. Oper Dent 2003;28:215-235.
Long-term durability of dentin bonds made with a self-etching primer, in vivo. J Dent Res 1999;78:906-911.
In vivo and in vitro permeability of one-step self-etch adhesives. J Dent Res 2004;83:459-464.
Single-step adhesives are permeable membranes. J Dent 2002;30:371-382.
Conversion of one-step to two-step self-etch adhesives for improved efficacy and extended application. Am J Dent 2005;18:126-134.
, Phark JH, Varjao FM, Sadan A. Nanoleakage, ultramorphological characteristics, and microtensile bond strengths of a new low-shrinkage composite to dentin after artificial aging. Dent Mater 2009;25:589-600.
Fluid movement across the resin-dentin interface during and after bonding. J Dent Res 2004;83:843-848.
Effect of various pretreatments for dentin bonding on dentin permeability. Shika Zairyo Kikai 1990;9:240-246.